many studies have been conducted on the long - term stability of osseointegrated dental implants.1 as dental implants have gained popularity , the necessity for bone grafts has become more prevalent . in many cases ,
the quantity of alveolar bone is often insufficient for the insertion of dental implant , because in many cases the tooth loss due to periodontitis or trauma is accompanied with alveolar bone loss . in addition , bone loss can occur due to peri - implantitis after implantation .
therefore , bone grafting procedures are becoming increasingly common.2,3 there are four classifications of bone graft materials .
these four types are known as autogenous bones , allogeneic bones , xenogeneic bones and alloplastic materials.4 among these materials , autogenous bones are the safest from immune rejection , but require additional surgical procedures for harvesting from donors .
allogeneic and xenogeneic bones require no additional procedures . however , there is a risk of disease transmission and it is impossible to adjust rates of biodegradation . on the other hands , for alloplastic materials , it is possible to regulate the rates of biodegradation and much easier to be sculpted into desired three dimensional forms.5,6 there have been several materials used for alloplastic materials .
hydroxyapatite ( ha ) , calcium phosphate , corals and bioglass are popular alloplastic bone graft materials.7 tricalcium phosphate ( tcp , ca3(po4)2 ) , which has a ca / p molar ratio of 1.5 has been used in clinical trials .
it has the crystal forms of alpha and beta , and  state shows greater microporosity and degradation than hydroxyapatite.8 ha is the most widely used material .
a molecular formula of ha is ca10(po4)6(oh)2 , and its ca / p ratio of 1.67 is most similar to the human bone structure .
the ha is an osteoconductive replacement material studied by numerous investigations , whether in vitro or in vivo .
the results from clinical trials have showed that ha is widely used clinically.9,10 biphasic calcium phosphate ( bcp ) is a mixture of tricalcium phosphate and hydroxyapatite .
researches have reported that bcps provide great biocompatibility and osteoconduction.11,12 in particular , mixtures of 40% -tricalcium phosphate ( -tcp ) and 60% hydroxyapatite produce better results than other compounds.13,14 alloplastic materials can be made in the desired three dimensional forms , including a porous structure .
the porous structure of bone graft materials is advantageous for the formation of new bone .
however , mechanical strength is a limiting factor in porous structures . in order to overcome this mechanical defect ,
porous scaffolds have been made of hard materials such as alumina or zirconia and coated with bioactive materials.15 hard scaffolds serve to maintain the volume of graft materials and therefore are useful in vertical bone augmentation .
zirconia adopts a tetragonal structure at high temperature and a monoclinic crystal at room temperature .
the volume expansion caused by cooling from high temperature results in cracking . in order to stabilize the tetragonal phase , zirconia is blended with a metal oxide such as yttria ( y2o3 ) .
, yttria stabilized tzp ( y - tzp ) has superior biocompatibility and mechanical properties in comparison to other tzps.16 accordingly , it has been used as a material in artificial joints for a long time.17,18,19 some studies on the biocompatibility of zirconia showed better results at osseointegration than titanium.20,21 due to these properties of zirconia , it is useful as a scaffold for bone graft material . while osseointegration and the mechanical properties of zirconia have been relatively much investigated , there are a few studies on the osteoblastic response of porous zirconia . in this study ,
the porous zirconia scaffolds coated with cap ceramics were fabricated using the powder slurry method .
the purpose of this study was to assess whether the coating procedures were adequate and to evaluate the biochemical properties of porous zirconia scaffolds coated with bioactive materials such as their dissolution behaviors . and
another aim of this study was to investigate the response of osteoblast - like cells cultured on the titanium and zirconia disks and porous zirconia scaffold by observing cell attachment and proliferation , and gene expression of the osteoblastic cell using mus musculus ( mouse ) calvaria derived osteoblast precursor cell ( mc3t3-e1 ) .
the titanium disks were fabricated from grade iv commercially pure titanium ( dynamet , carpenter technology co. , washington , pa , usa ) , 8 mm in diameter and 4 mm in thickness .
pre - sintered zirconia blocks ( lava zirconia block , 3 m espe , neuss , germany ) were designed and sintered to be 8 mm in diameter and 4 mm in thickness .
an open cell polyurethane disk foam template ( 10 mm  5 mm , 60 ppi , filtrocell , eurofoam , troisdorf , germany ) was used to fabricate a porous scaffold .
the polyurethane foam was dipped in 2% naoh solution for 30 minutes and washed with distilled water and dried at room temperature for 24 hours .
100 g of zro2 powder ( tz-3y - e , tosoh co. , yamaguchi , japan ) calcined at 600 for 2 hours and 6 g of triethyl phosphate ( tep ) were mixed in ethanol for 24 hours by a ball mill .
pretreated polyurethane foams were dipped and compressed several times in the slurry . and residual slurry was removed by using at low speed by centrifuge .
after this procedure was repeated two times , the coated foams were dried at room temperature for 24 hours .
the coated foams were sintered at a heating ratio of 1/min to 600 , and then maintained at 600 for 2 hours in order for the polyurethane foams to be burnt out .
after that , heat - treatment was performed at a heating ratio of 3/min to 1550 for solidification .
louis , mo , usa ) , ha powders ( hydroxyapatite , sigma - aldrich corp . , st .
louis , mo , usa ) , and a compound of -tcp and ha powders were mixed in the ratio of 40 to 60 were calcined at 600 for 2 hours .
25 g of each powder and 4 g of tep were added to the powder mixture in ethanol for 24 hours by a magnetic stirrer .
the slurry was completed by adding 4 g of pvb , and then stirring for 24 hours .
the pretreated zirconia scaffolds were dipped in the slurry and residual slurry was removed by air gun .
after this procedure was repeated twice , the coated scaffolds were dried at room temperature for 24 hours .
the coated scaffolds were heat - treated at a heating ratio of 3/min to 1200. after sustaining a temperature of 1200 for 2 hours for the purpose of solidification , the coated zirconia scaffolds were slowly cooled .
all samples were ultrasonically cleaned using an ethanol for 10 minutes , washed in running water and finally rinsed in distilled water and dried .
the titanium disks , zirconia disks and coated zirconia scaffolds were evaluated by using scanning electron microscope ( mira lmh , tescan , brno , czech republic ) and energy dispersive x - ray spectrometer ( xflash detector 5010 , brunker , fitchburg , wi , usa ) .
the crystallography of the specimens was analyzed by x - ray diffractometry ( xrd ) in an x - ray diffractometer ( minifelx600 , rigaku , tokyo , japan ) .
the range of 2 was from 10 to 70 with a scanning rate of 1/min .
the coated zirconia scaffolds were immersed in a 10 ml 0.03 m tris - buffer solution ( tris(hydroxyl)methyl - aminomethane with hydrochloric acid , t&i co. , gangwon , korea ) at ph 7.0 .
these buffer solutions were kept to 37 by placing them in a water bath ( wisebath , daihan scientific co. ltd . ,
the calcium and phosphorus ion concentration of buffer solutions were measured by an inductively coupled plasma spectrometer ( icp ) ( icap6300 , thermo scientific , waltham , ma , usa ) .
mc3t3-e1 preosteoblastic cells ( atcc cell bank , manassas , va , usa ) were cultured in normal media containing dulbecco 's modified eagle medium high glucose ( dmem)(gibco , grand island , nj , usa ) supplemented with 10% heat - inactivated fetal bovine serum ( fbs ) ( cellect gold , mp biomedicals , irvine , ca , usa ) , 100 u / ml of penicillin and 10 g / ml of streptomycin , and maintained at 37 in an atmosphere of 5% co2 .
the attachment and proliferation of mc3t3-e1 cells was determined trypsinizing and cell counting by using a hemocytometer .
the mc3t3-e1 cell was seeded onto the disk and scaffold at a density of 1  10 cells / ml and cultured for 4 hour and 5 days .
the osteoblastic differentiation of mc3t3-e1 cell was evaluated by a reverse transcriptase - polymerase chain reaction ( rt - pcr ) analysis of type i collagen ( col1a1 ) , osterix , osteocalcin(ocn ) , alkaline phosphatase ( alp ) , runx2 and -actin .
the cells were plated at a density of 1  10 cells / ml on disks and scaffolds .
the total rna was isolated from the cultures using the trizol reagent ( invitrogen , carlsbad , ca , usa ) according to the manufacturer 's instructions .
the total rna was used for cdna synthesis by reverse transcriptase with cdna synthesis kit ( gibco , grand island , nj , usa ) .
detection of the pcr amplicons was operated by size fractionation by 1% ( w / v ) agarose gel electrophoresis .
surfaces were analyzed using scanning electron microscope ( sem ) to determine their cellular morphology .
mc3t3-e1 cell suspension ( 3  10 cells / ml ) was seeded to disks and scaffolds and samples were observed after 3 and 7 days .
after levene 's test was performed to confirm equal variance assumption , an analysis of variance ( anova ) was conducted to assess the statistical significance of the differences , followed by scheff 's multiple comparison test , which was done to assess the presence of significant differences ( ibm - spss statistics 21 , ibm - spss inc . ,
sem images of titanium disk showed concentric micro - groove patterns form machining , but there was no crystalline structure .
similarly , sem images of zirconia disk showed irregular micro - groove patterns from grinding before sintering .
the crystalline structure of ha appeared to have a smaller size than -tcp ( fig .
spectrum of zirconia disk and zirconia scaffold showed not only zirconium but also yttrium . from the edx profiles ,
the results of edx confirmed that one was crystal of -tcp and the other was crystal of ha ( table 2 ) .
xrd patterns of zirconia scaffold with -tcp , ha and bcp coating were obtained ( fig .
the peaks observed at 27.8 , 31 and 34.4 were attributed to the -tcp cultured in static circumstance .
the amount of dissolved ca ions in the solution was different depending on the coating materials .
also , more ca ion was observed on the bcp coated zirconia scaffold than on the ha coated zirconia scaffold .
the differences were statistically significant ( p<.05).the ca / p ratio in the solution was different depending on the coating materials ( table 3 ) .
after 4 hours of cell seeding , there was no significant difference in all groups .
the cell proliferation of titanium disk appeared significantly lower in comparison with other groups ( p<.05 ) .
the cell density on zirconia scaffolds with or without coating showed no significant difference , but was significantly higher than on the zirconia disk ( p<.05)(fig .
4 ) . after incubation of osteoblastic cells for 1 day , the mrna expression of type i collagen , runx2 , osterix on all groups showed similar activity .
the level of alp mrna expression increased at 2 days on zirconia disk while it increased at 3 days on the titanium disk .
mrna expression of alp on zirconia scaffold based group were observed at 1 day . the mrna level of osteocalcin was higher on non - coated zirconia scaffold compared with the other groups at 7 days ( fig . 5 ) .
after 3 days of cell culture , the mc3t3-e1 cells on the titanium disks were observed flat .
sem images of zirconia disk showed that cells were convex in comparison to these on the titanium disks .
cells on coated zirconia scaffolds had spindle shape morphology when compared with other samples , but did not have well - developed filopodias ( fig .
after 7 days of cell culturing , a number of cells on the titanium disk were showed flat and spread out .
the cells on the zirconia disk were similar to these on the titanium disk , but the number of cells was more than on titanium disk .
mc3t3-e1 cells on coated zirconia scaffolds had several short filopodias ( fig . 7 ) .
since crystalline bone screws were first made of aluminum oxide in 1968 , many ceramic implants have been commercialized.22,23 various kinds of ceramics have been used for osseointegration of implants but have some limitation due to their physical properties.24 on the other hand , yttriumoxide partially stabilized zirconia ( y - psz ) or yttrium - tetragonal zirconia polycrystals ( y - tzp ) can be used as a biomaterial with good biocompatibility and high fracture strength .
recently , titanium has been used as a non - absorbable bone graft material.25 it is used for bone grafting during implant placement as well as recovering bone volume for the treatment of peri - implantitis , because it can maintain the stable volume of bone.26 the advantage of zirconia over titanium is that it is a bioinert material with a non - metallic color and good biocompatibility.27 as with titanium , zirconia performs better osseointegration in comparison to other materials , because it does not interfere with the growth of osteoblasts.18 in this study , cells cultured on the titanium disks showed similar initial adhesion properties to the zirconia disks .
however , the zirconia disks had a significantly greater positive effect on the proliferation of osteoblasts .
furthermore , the gene expression analysis of the mc3t3-e1 cells showed that the differentiation potency of the cells cultured on the zirconia disks was better than that on the titanium disks .
langhoff et al.28 reported that bone to implant contact of zirconia was significantly greater than that of titanium .
the surface treatment of titanium is relatively a simple process , which makes the material popular .
but in the case of zirconia , the surface treatment is rarely used because the surface treatment is difficult .
the sintering process is the most common method for fabricating porous scaffolds.21 for the growth of osteoblast , porous surfaces is critical , because cells are attached to the pore and can spread through interconnected pore .
therefore , the activity of osteoblast is better on porous surfaces than on simple rough surface .
the pore size is also important and the optimal pore size for osteoblast activity is 100 - 400 m.29 in this study , the sem micrographs showed that the pore size of the zirconia scaffolds was 200 500 m .
the cell proliferation of the zirconia disks was significantly lower than that of the zirconia scaffolds .
as one of the methods for fabricating porous zirconia scaffolds , zirconia powders are mixed with the substances that vaporize relatively at low temperature .
this method is very simple but it is impossible to make well - formed interconnecting pores.30 the method of coating open cell sponge foams after sintering was difficult to perform due to sintering temperature and coating process .
the second process is a differentiation of cells , which is the process of qualitative growth . during the initial stage of cell attachment
the surfaces were coated with small crystals of ha , and then -tcp in bcp coating .
the -tcp coating had the largest amount of dissolved ca ions due to its higher solubility than ha .
the ca / p ratio in the solution was different depending on the coating materials . because the zirconia scaffold is an inert material , it showed the ca / p ratio of the coating materials .
the ca / p ratios of the zirconia scaffold in the solution of -tcp , ha and bcp coating were 1.52 , 1.68 and 1.63 respectively , which were similar to those of -tcp , ha and bcp ( 1.5 , 1.67 and 1.608 ) .
the ca / p ratios of -tcp and ha were 1.53 and 1.68 , and consistent with those of icp analysis .
the ca / p ratio in the solution of bcp coating was not statistically significant .
as in the sem micrograph of bcp coating , the crystal of ha was greater than that of -tcp .
a mc3t3-e1 mouse pre - osteoblastic cell was used for this study due to its high level of differentiation and its ability to confirm bone markers such as type i collagen , osterix , osteocalcin , alp and runx2 , making it an excellent model for cell differentiation.31,32 type i collagen is a major extracellular matrix of fibroblasts.33 osterix is an essential transcription factor for osteoblast differentiation .
osteocalcin is an osteoblast - specific protein and is secreted by osteoblasts to play a role in the metabolic regulation of calcium ion.34 runx2 is the best known as a key regulator of osteoblast marker genes .
runx2 can also directly stimulate the transcription of osteoblast - related genes such as those encoding osteocalcin ( ocn ) , type i collagen , osteopontin ( opn).35 the mrna levels of -actin , commonly called housekeeping gene , served as a control .
the coated scaffold was partially obturated as compared to the non - coated zirconia scaffold in sem micrographs . during the coating process
however , it was difficult to remove all of the coating materials at the bottom .
because the solvent of the slurry of coating materials was evaporated quickly by using an air gun , it was considered that coating materials remained interporous .
there was no difference in cell proliferation between non - coated scaffolds and coated scaffolds .
no difference in cell attachment and proliferation was observed despite partial obturation of interconnecting pores , but the activity of cell differentiation was greater in non - coated zirconia scaffolds with interconnecting pores .
after 7 days in the cultures , the mrna expression of osteocalcin was distinctly detected only in the non - coated zirconia scaffolds .
therefore , the differentiation of osteoblast cells was influenced by microstructure rather than coating material.36 it is concluded that the activity of osteoblast in zirconia was higher than in titanium .
the results of this study showed that the non - coated zirconia scaffold was superior .
it was found from the results that the activity of osteoblasts was more affected by microstructure than coating material .
the limitation of this study was that it was at the cellular level for a short term , and that the coating material obturated interconnecting pore partially .
for the commercialization of a zirconia bone graft , a proper coating method should be used in order to ensure optimal osteogenic process while maintaining interconnecting pores .
in addition , there is a need for further in vivo studies to make improvement in material properties .
based on the results of this study , the osteoblast cell activity on zirconia was higher than on titanium .
further research is required to investigate the influence of coating materials and microstructures such as interconnecting pore on differentiation of osteoblast in a tightly controlled environment .
 purposethe purpose of this study was to evaluate the properties of a porous zirconia scaffold coated with bioactive materials and compare the in vitro cellular behavior of mc3t3-e1 preosteoblastic cells to titanium and zirconia disks and porous zirconia scaffolds.materials and methodstitanium and zirconia disks were prepared . 
 a porous zirconia scaffold was fabricated with an open cell polyurethane disk foam template . 
 the porous zirconia scaffolds were coated with -tcp , ha and a compound of -tcp and ha ( bcp ) . 
 the characteristics of the specimens were evaluated using scanning electron microscopy ( sem ) , energy dispersive x - ray spectrometer ( edx ) , and x - ray diffractometry ( xrd ) . 
 the dissolution tests were analyzed by an inductively coupled plasma spectrometer ( icp ) . 
 the osteogenic effect of mc3t3-e1 cells was assessed via cell counting and reverse transcriptase - polymerase chain reaction ( rt - pcr).resultsthe edx profiles showed the substrate of zirconia , which was surrounded by the ca - p layer . in the dissolution test , dissolved ca2 + ions were observed in the following decreasing order ; -tcp > bcp > ha ( p<.05 ) . in the cellular experiments , the cell proliferation on titanium disks appeared significantly lower in comparison to the other groups after 5 days ( p<.05 ) . 
 the zirconia scaffolds had greater values than the zirconia disks ( p<.05 ) . 
 the mrna level of osteocalcin was highest on the non - coated zirconia scaffolds after 7 days.conclusionzirconia had greater osteoblast cell activity than titanium . 
 the interconnecting pores of the zirconia scaffolds showed enhanced proliferation and cell differentiation . 
 the activity of osteoblast was more affected by microstructure than by coating materials . 
INTRODUCTION
MATERIALS AND METHODS
RESULTS
DISCUSSION
CONCLUSION